Designation: C 1105 – 05
Standard Test Method for
Length Change of Concrete Due to Alkali-Carbonate Rock Reaction 1 This standard is issued under the ﬁxed designation C 1105; the number immediately following the designation indicates the year of original adoption or, in the case of revision, the year of last revision. A number in parentheses indicates the year of last reapproval. A superscript supers cript epsilon (e) indicates an editorial change since the last revision or reapproval.
1. Sco Scope pe
C 511 Speciﬁ Speciﬁcati cation on for Mixi Mixing ng Rooms Rooms,, Mois Moistt Cabin Cabinets, ets, Mois Mo istt Ro Room oms, s, an and d Wat ater er St Stor orag agee Tan anks ks Us Used ed in th thee Testing of Hydraulic Cements and Concretes C 586 Test Method for Potential Alkali Reactivity of Carbonatee Rocks for Concr bonat Concrete ete Aggregates Aggregates (Rock Cylinder Method) C 595 Speciﬁcation for Blended Hydraulic Cements C 670 Practice for Preparing Precision Statements for Test Methods for Construction Materials C 702 Practice for Reducing Field Samples of Aggregate to Testing Size D 75 Practice for Sampling Aggregates
1.1 This test method covers covers the determination, determination, by measurement of length change of concrete prisms, the susceptibility of cement-aggregate combinations to expansive alkali-carbonate reaction react ion invol involving ving hydr hydroxide oxide ions asso associat ciated ed with alka alkalies lies (sodium (sodi um and potas potassium) sium) and cert certain ain calci calcitic tic dolom dolomites ites and dolomitic limestones. 1.2 The values values stated in SI units are to be regarded regarded as the standard. standard d doe doess not purport purport to add addre ress ss all of the 1.3 This standar safe sa fety ty co conc ncer erns ns,, if an anyy, as asso soci ciat ated ed wit with h its us use. e. It is th thee responsibility of the user of this standard to establish appro priate safety and health practices and determine the applicability of regulatory limitations prior to use.
3. Terminology 3.1 Termi erminolog nology y used in this standard standard is deﬁne deﬁned d in TermiTerminology C 125 or nology C 125 or Descriptive Nomenclature C 294. 294.
2. Referenced Documents 2.1 ASTM Standards: 2 C 33 Speciﬁcation for Concrete Aggregates C 125 Term Termino inolog logy y Rel Relati ating ng to Con Concre crete te and Con Concre crete te Aggregates C 150 Speciﬁcation for Portland Cement C 157/C 157M Test Test Method for Lengt Length h Chang Changee of Hardened Hydraulic-Cement Mortar and Concrete C 233 Test Method for Testing Air-Entraining Admixtures for Concrete C 294 Descriptive Descriptive Nomenclature Nomenclature of Const Constitue ituents nts of Concrete Aggregates C 295 Guide for Petro Petrograph graphic ic Exami Examinati nation on of Aggregates Aggregates for Concrete C 490 Practice for Use of Apparatus for the Determination of Length Change of Hardened Cement Paste, Mortar, and Concrete
4. Signi Signiﬁcanc ﬁcancee and Use 4.1 Two types of alka alkali li reactivity reactivity of aggre aggregates gates have been described in the literature: the alkali-silica reaction involving certain siliceous rocks, minerals, and artiﬁcial glasses ( (1 1),3 and the alka alkali-c li-carbon arbonate ate react reaction ion invol involving ving dolom dolomite ite in cert certain ain calcitic calc itic dolo dolomite mitess and dolom dolomitic itic lime limeston stones es (2). Th This is te test st method is not recommended as a means to detect combinations susceptible to expansion due to alkali-silica reaction since it was not evaluated for this use in the work reported by Buck ( Buck (2 2). This test method is not applicable to aggregates that do not contain or consist of carbonate rock (see Descriptive Nomenclature C clature C 294). 294). 4.2 This test method is intended for evaluating evaluating the behavior of speci speciﬁc ﬁc combi combinati nations ons of conc concreterete-maki making ng mate material rialss to be used in the work. However, provisions are made for the use of substitute materials when required. This test method assesses the pot potent ential ial for exp expans ansion ion of con concre crete te cau caused sed by alk alkali ali-carbonate rock reaction from tests performed under prescribed laboratory curing conditions that will probably differ from ﬁeld
Thiss test method is und Thi under er the jurisdicti jurisdiction on of ASTM Com Commit mittee tee C09 on Concrete and Concrete Aggregates and is the direct responsibility of Subcommittee C09.26 on Chemical Reactions. Curren Cur rentt edit edition ion app approv roved ed May 1, 200 2005. 5. Pub Publish lished ed May 200 2005. 5. Ori Origin ginally ally approved approv ed in 1989. Last previous edition approved in 2002 as C 1105 – 95(2002 95(2002). ). 2 For referenced ASTM standards, visit the ASTM website, www.astm.org, or contact ASTM Customer Service at [email protected] [email protected]
astm.org. g. For For Annual Annual Book of ASTM Standards volume information, refer to the standard’s Document Summary page on the ASTM website website..
The boldface boldface numbers in parentheses parentheses refer to the list of references at the end of this test method.
Copyright © ASTM International, 100 Barr Harbor Drive, PO Box C700, West Conshohocken, PA 19428-2959, United States.
C 1105 – 05 conditions. Thus, actual ﬁeld performance will not be duplicated due to differences in wetting and drying, temperature, other factors, or combinations of these (see Appendix X1). 4.3 Use of this test method is of particular value when samples of aggregate from a source have been determined to contain constituents that are regarded as capable of participation in a potentially deleterious alkali-carbonate rock reaction either by petrographic examination, Guide C 295, by the rock cylinder test, Test Method C 586, by service record; or by a combination of these. 4.4 Results of tests conducted as described herein should form a part of the basis for a decision as to whether precautions be taken against excessive expansion due to alkali-carbonate rock reaction. This decision should be made before a particular cement-aggregate combination is used in concrete construction (see Note 1).
184.108.40.206 In the case of construction where several size ranges coarser than the 19.0-mm ( 3 ⁄ 4-in.) sieve are contemplated, each of these may, if desired, be separately crushed to pass this sieve and may be tested separately. 6.2 Job Cement —When it is desired to evaluate a particular cement-aggregate combination for use in particular work, the cement or cements used shall meet the requirements for the work and shall be from the source or sources and in the amounts expected to be used in the work. If several cements may be used in the work, it is desirable that tests be made using each cement separately. 6.3 Reference Cements—When it is desired to evaluate aggregates for general use or to compare aggregates for investigational purposes, the cement used shall be of the highest alkali content representative of the general use intended, or available to the laboratory making the tests. The cement or cements selected should comply with Speciﬁcation C 150 or Speciﬁcation C 595. Additional information of value may be obtained by conducting parallel tests with cements of different alkali content, of different sodium oxide to potassium oxide ratio, or blended with pozzolan or ground blast-furnace slag, or both. 6.4 Substitute Fine Aggregate—If the test aggregate is to be used only as coarse aggregate and the ﬁne aggregate that it will be used with is not available, a ﬁne aggregate that is not expected to participate in an expansive reaction with alkalies (see Note 2) shall be used.
NOTE 1—Other elements that may be included in the decision-making process for categorizing an aggregate or a cement-aggregate combination with respect to whether precautions are needed, and examples of precautions that may be taken, are described in Appendix X1.
4.5 While the basic intent of this test method is to develop information on a particular cement-aggregate combination, it will usually be very useful to conduct control tests in parallel using the aggregate of interest with other cements or the cement of interest with other aggregates. 5. Apparatus 5.1 The mold, the associated items for molding test specimens, and the length comparator for measuring length change shall conform to the applicable requirements of Test Method C 157/C 157M and Practice C 490.
NOTE 2—Advice on judging the expansive reactivity of aggregate is given in Appendix XI of Speciﬁcation C 33.
7. Sampling 7.1 Obtain the sample in accordance with Practice D 75 and reduce it to test portion size in accordance with Practice C 702.
6. Materials 6.1 Maximum Size of Coarse Aggregate —Coarse-aggregate fractions larger than the 19.0-mm ( 3 ⁄ 4-in.) sieve shall not be tested as such. When petrographic examination using Guide C 295 reveals that the material making up the size fractions larger than the 19.0-mm sieve is of such a composition and lithology that no differences should be expected compared with the smaller size material to be tested, or when tests, made in accordance with Test Method C 586, of material in such sizes reveal no signiﬁcant differences from the sizes to be tested, then no further attention need be paid to the larger sizes. If results of petrographic examination or tests made in accordance with Test Method C 586 suggest that the larger size material should be studied for its effects in concrete, one or the other of two alternative procedures described herein may be used. 6.1.1 Proportional Testing—Material larger than the 19.0-mm (3 ⁄ 4-in.) sieve shall be crushed to pass the 19.0-mm sieve and material larger than the 4.75-mm (No. 4) sieve shall be proportioned to include the same proportion by mass of the crushed material originally retained on the 19.0-mm sieve and that originally passing this sieve, as may be expected to be used in the ﬁeld concrete. 6.1.2 Separated Size Testing—Material larger than the 19.0-mm (3 ⁄ 4-in.) sieve shall be crushed to pass this sieve and shall be used in concrete as a second aggregate.
8. Test Specimens 8.1 Prepare six specimens, of the type required for concrete Test Method C 157/C 157M, having square cross-sections of 75.0 6 0.7 mm or 3.00 6 0.03 in. from one batch of concrete. The concrete mixture shall be the mixture in which the aggregates are proposed for use. In the event that no speciﬁc concrete mixture is being considered, that described in Test Method C 233 may be used. 8.2 If control or comparison mixtures are made, specimens shall be made from those mixtures as described in 8.1. 9. Conditioning 9.1 Cure, store, and remove molds in accordance with Test Method C 157/C 157M. Thereafter, keep the specimens in moist storage in accordance with Speciﬁcation C 511 but do not immerse in water. 10. Procedure 10.1 Follow the procedure of Test Method C 157/C 157M, except that the specimens shall be stored in a moist room or moist cabinet meeting the requirements of Speciﬁcation C 511 and length measurements shall be made at ages 7, 28, and 56 days, and 3, 6, 9, and 12 months. 2
C 1105 – 05 11. Calculation
Average % Expansion